107KONICA TECHNICAL REPORT VOL.162003
Ink Jet Technology DivisionCorporate Technology Center
A Pigment Precursor for Inkjet Inks
Ohya, HidenobuKida, ShujiAbe, Takao
There are two general categories of water-based inkjet inks: dye-based inks and pigment-based inks. Pig-
ment-based inks provide images with comparatively greater stability when subjected to light or to chemically
reactive materials such as oxidizing gases. However, pigment-based inks typically fail to provide image gloss
and resistance to abrasion. In response, we have developed a novel inkjet ink that employs a new water-
soluble pigment precursor. During printing, this pigment precursor ink behaves much like a dye-based ink. But
once this ink has been applied to the print medium, a simple treatment triggers the provision of pigment
particles. The result is an image that possesses not only high image stability but also high gloss and high
resistance to abrasion.
Recent years have seen marked technical advances in
inkjet printing, with the image quality and the image
stability of inkjet prints approaching those of photographic
Many efforts that have borne on bringing high image
quality and high image stability together have been made.
Bauer, Baumgart, and Zoller surveyed a number of wa-
ter-soluble magenta dyes. Bugner and Burmel studied
the effect of particle size in pigment inks on such charac-
teristics as printing reliability, image quality, and dura-
bility. Tsutsumi, Sawada, and Nakano developed an
emulsion colorant involving a water-based polymer emul-
sion that contained a water-insoluble dye or pigment.
Zhimin and Abul developed a solvent-soluble pigment
precursorlatent pigments. And Parazak examined
the application of latent pigments to inkjet printing .
We join these efforts with a method in which a water-
soluble pigment precursor penetrates the surface of the
printing medium and then releases a pigment. This com-
bines the high gloss and resistance to abrasion of a dye-
based ink with the superior light stability of a conven-
tional pigment-based ink.
Our work may be viewed in four segments:
1. The design and synthesis of a new water-soluble
2. The preparation of an ink containing that water-
soluble pigment precursor, and printing an interim
image with that ink,
3. The post-printing treatment of the medium to re-
lease the pigment from the pigment precursor, and
4. The evaluation of the terminal image.
Design and synthesis of pigment precursor
We selected a quinacridone pigment CI Pigment Red
122 as our color material because magenta presents the
greatest challenge to simultaneously achieving optical
brightness and high image stability.
Fig.1 Pigment precursor
In the pigment precursor that we designed and syn-
thesizedFig. , the nitrogen atomsAare protected
by groupsBto increase water solubility, which is ac-
complished by preventing the aggregation of molecules.
The groups contain a water-soluble radicalC. The
composition of the groupsBis designed to afford ease
of synthesis and stability in water. Compared to an m-
sulfonic acid salt type, this o-sulfonic acid salt type pre-
cursor is easy to synthesize and provides good stability;
in this, the steric effect of the o-sulfonic acid salt is likely
The pigment precursor was synthesized from CI Pig-
108 KONICA TECHNICAL REPORT VOL.162003
ment Red 122 and o-sulfobenzoic anhydride, using NaH
in HMPA or N-methylpyrolidoneFig. . The com-
pound obtained was identified as the target compound
through NMR and mass spectra.
The pigment precursor was dissolved in water to ap-
proximately a 10% solution, the solution was colored yel-
low, and the stability of the pigment precursor was then
studied at various pH values. The pigment precursor
was stable in alkali Fig. and neutral conditions,
while in acidic conditionsin a pH 1.68 buffer, the pre-
cursor was slowly hydrolyzed at room temperature, and
a red precipitate appeared.
Fig.3 Stability of the pigment precursorpH10.0
Fig.2 Synthesizing the pigment precursor
Ink preparation and printing
We prepared an ink containing the pigment precur-
sor, consisting of the following:
Triethylene glycol mono-n-butyl ether (10%)
With this ink, we printed on a porous mediumKonica
Inkjet Paper Photolike QP with a commercial inkjet printer
Piezo typeand obtained a yellow imageFig. .
Prints were sprayed with diluted sulfuric acid or p-
toluene sulfonic acid aqueous solution, and heated to 90-
130 for several seconds with a commercial laminator.
This post-printing treatment caused the pigment pre-
cursors to be hydrolyzed and thus to release the pig-
ment particlesFig. . Consequently, from the yel-
lowish, interim image, the reddish, terminal image
Fig.4 Synthesizing the pigment precursor
109KONICA TECHNICAL REPORT VOL.162003
Evaluation the image
We measured the reflection spectra of the terminal
image and compared it with that of an image printed
with conventional CI Pigment Red 122 water-based ink
Fig. . The two spectra were nearly identical.
Fig.5 Reflection spectra
Extending our comparison to encompass an appropri-
ate dye image, we evaluated the gloss, light stability, and
resistance to abrasion resultant from the three types of
inksTable. The pigment precursor image exhib-
ited the high gloss and resistance to abrasion of the dye
image while it approached the light stability of the con-
ventional pigment image.
Table1 Image evaluations
To determine how the pigment precursor image man-
aged to simultaneously avoid the low gloss and resistance
to abrasion of the conventional pigment image and the
low light stability of the dye image, we examined micro-
scopic, cross-sectional views of each imageFig. .
Pigments naturally provide high light stability. How-
ever, with a conventional pigment imageFig.A,
the pigment lies chiefly on the surface of the medium.
Because the average size of the pigment particle is
roughly 100-150nm, the pigment particle is prevented
from penetrating the surface. The result is a surface
roughness that both limits gloss and leaves the image
susceptible to abrasion.
In contrast, dye imagesFig.B, by their nature,
do not provide sufficient light stability. However, because
dye images penetrate the surface of the medium, they
do allow high gloss and high resistance to abrasion.
In the pigment precursor imageFig.C, the pig-
ment precursor deposits the pigment well below the sur-
face of the medium; thus, just as with dyes, gloss and
resistance to abrasion are high. But at the same time, by
virtue of being true pigments, light stability is also high.
It should be observed that the light stability of our
experimental pigment precursor images, while exhibit-
ing the characteristically superior light stability of a pig-
ment image, does not yet match the performance of a
conventional pigment-based inkFig. . As we ad-
dress this challenge, we note that the light stability of a
pigment image generally increases with the size of the
Fig.6 Light stability
110 KONICA TECHNICAL REPORT VOL.162003
We synthesized a quinacridone type water-soluble pig-
ment precursor and evaluated its performance. Our re-
sults indicate that inkjet inks using pigment precursors
promise to combine the high gloss and resistance to abra-
sion of dye-based inks with the high light stability of
conventional pigment inks.
Wolfgang Bauer, Dieter Baumgart, and Walter Zoller, IS&T's
NIP12: International Conference on Digital Printing Technolo-
gies, Proceedings, pp.59-65 (1996)
D.E. Bugner and A.D. Bermel, IS&T's NIP13: International Con-
ference on Digital Printing Technologies, Proceedings, pp.667-
T. Tsutsumi, M. Sawada, and Y. Nakano, IS&T's NIP15: Inter-
national Conference on Digital Printing Technologies, Proceed-
ings, pp.133-136 (1999 )
Hao Zhimin and Iqbal Abuul, United States Patent No.5591865,
5616725, 5646299, and 5650520
Dennis P. Parazak, Japanese Patent Publication Open to Public
Inspection No. 11-246809
Fig.7 Cross-sectional views of images